energies Article Study of Dielectric Breakdown Performance of Transformer Oil Based Magnetic Nanofluids Yuzhen Lv ID , Muhammad Rafiq *, Chengrong Li and Bingliang Shan Beijing Key Laboratory of High Voltage & EMC, North China Electric Power University, Beijing 102206, China; email@example.com (Y.L.); firstname.lastname@example.org (C.L.); email@example.com (B.S.) * Correspondence: Jutt96@gmail.com; Tel.: +86-10-61772352 Received: 21 March 2017; Accepted: 10 July 2017; Published: 19 July 2017 Abstract: Research on the transformer oil-based nanofluids (NFs) has been raised expeditiously over the past decade. Although, there is discrepancy in the stated results and inadequate understanding of the mechanisms of improvement of dielectric nanofluids, these nanofluids have emerged as a potential substitute of mineral oils as insulating and heat removal fluids for high voltage equipment. The transformer oil (TO) based magnetic fluids (ferrofluids) may be regarded as the posterity insulation fluids as they propose inspiring unique prospectus to improve dielectric breakdown strength, as well as heat transfer efficiency, as compared to pure transformer oils. In this work, transformer oil-based magnetic nanofluids (MNFs) are prepared by dispersal of Fe3 O4 nanoparticles (MNPs) into mineral oil as base oil, with various NPs loading from 5 to 80% w/v. The lightning impulse breakdown voltages (BDV) measurement was conducted in accordance with IEC 60897 by using needle to sphere electrodes geometry. The test results showed that dispersion of magnetic NPs may improve the insulation strength of MO. With the increment of NPs concentrations, the positive lightning impulse (LI) breakdown strength of TO is first raised, up to the highest value at 40% loading, and then tends to decrease at higher concentrations. The outcomes of negative LI breakdown showed that BDV of MNFs, with numerous loadings, were inferior to the breakdown strength of pure MO. The 40% concentration of nanoparticles (optimum concentration) was selected, and positive and negative LI breakdown strength was also further studied at different sizes (10 nm, 20 nm, 30 nm and 40 nm) of NPs and different electrode gap distances. Augmentation in the BDV of the ferrofluids (FFs) is primarily because of dielectric and magnetic features of Fe3 O4 nanoaprticles, which act as electron scavengers and decrease the rate of free electrons produced in the ionization process. Research challenges and technical difficulties associated with ferrofluids for practical applications are mentioned. The advantages and disadvantages linked with magnetic fluids are also presented. Keywords: breakdown strength; nanoparticles; nanofluids; dielectric improvement; transformers 1. Introduction The evolution of prospective high voltage systems and smart grids has placed significant demands on the reliability and conduct of insulating materials applied in electric power networks to cope with vital and volatile operating conditions . An essential component of electrical networks which alters voltage levels and transforms energy is called a transformer . The majority of transformer units in operation across the world are near or beyond their design life; thus, it has been a major aim to enhance the operational reliability of the existent entities . The high voltage (HV) machinery collapse statistics illustrated that usual service life of transformers, which collapse due to insulation complications, is 17.8 years, which is half of their anticipated life of 35 to 40 years  and 75% of transformer failures are mainly caused by insulation issues . The status and properties of insulation materials are very important for the functional reliability and lifetime of transformers [5–8]. Energies 2017, 10, 1025; doi:10.3390/en10071025 www.mdpi.com/journal/energies Energies 2017, 10, 1025 2 of 21 Mineral oil and cellulose insulation systems have been successfully applied in the transformer industry over the last century. The rise in system voltage levels with recent developments has put a continuous pressure on these insulation systems to meet the demands of high reliability, high tolerance to field strength and smaller size. Nevertheless, in oil/cellulose insulation, the disparity between liquid permittivity (~2.2) and a solid one (ranging, 3.6~4.5) has been a serious concern that might confine the compact design of high voltage machinery, since the liquid undergoes a higher stress than the solid at alternating current (AC) and/or impulse voltages. Whereas, the BD strength of the liquid is basically less than that of the solid. The insulation liquid basically executes two primary actions in high voltage equipment: insulation and cooling. Insulating and thermal features of mineral oil typically restrain the minimal size and maximal transfer of power [9,10]. Nonetheless, the greatly refined mineral oils (MOs) commonly employed as insulation liquids in high voltage apparatus, possess low thermal conductivity and thus, achieve low cooling efficiency . Transformer oil is one the most significant elements of the transformer, which executes the aforementioned two major functions: as a cooling fluid, it is helpful in transferring the heat produced in the active parts (windings and magnetic core) to the tank walls of the transformer, where it may be exhausted; as an insulating material, the oil hinders the flow of electric current outside of the electric elements . The low thermal conductivity of transformer oil (TO) causes restraints in the conduct of transformers, because of conditions such as over loading and extreme rise in temperatures causing enormous local increase in temperature in the oil (hotspot), so that the efficiency of the TO is restricted. Refining the inquiry of materials down to the nanometer scale frequently shows new characteristics of matter that have no equivalent on a large scale. This phenomenon is encouraging in many current investigations of nanomaterials, which can disclose some new interesting phenomena. Fluids with suspended nanoparticles (NPs) (of a few tens of nanometers) well distributed in liquids are noted as nanofluids (NFs), a word suggested by Choi et al. , denoting the suspension of fine particles in a host liquid with no significant sedimentation of particles over time . In addition to MOs, other inorganic and organic liquids have been applied as the matrix for nanofluids development. The nanoparticles with a larger surface area, as compared with ordinary particles, do not only considerably enhance transfer capacity, but also boost the stability of the suspensions . Liquid or solid insulators, integrating within their volumes suspended NPs, manifest appealing permittivity traits, with supplementary polarization mechanisms evolving across the interface of the matrix material and distributed particles. Nanofluids can be considered as two-phase systems, the one phase being the matrix and the other being the scattered NPs. Materials applied to nanofluids formation include metals, metal oxides and nitrides. Accordingly, the resulting fluid may display different conductivities and/or permittivities. NFs have been found to have upgraded thermo-physical features e.g., thermal conductivity, viscosity, thermal diffusivity and convective heat transfer coefficients, as compared to those of carrier liquids. It has displayed significant potential applications in various fields. The biggest issues being faced by this two-phase system is the stability of NFs; there is as of yet, no clear way to stabilize NFs to the required levels. Nanofluids are being discussed as the future-era heat transfer liquids, because they show overwhelming potential to enhance heat transfer conduction, as compared to base liquids . Different nanoparticles Fe3 O4, TiO2 and Al2 O3 can upgrade the breakdown voltage (BDV) of TO. Nevertheless, magnetic NPs (Fe3 O4 ), that is, a type of well-known nanoparticles in multiple research areas such as chemistry, biology and applied physics [15–18]. They can also improve the heat transfer by thermo-magnetic convection, due to magnetic characteristics of Fe3 O4 , which has significant advantages for the cooling of the transformer . They are ferromagnetic materials and have strongest magnetism between iron oxides. Colloids consisting of magnetic nanoparticles (magnetite) coated surfactants and suspended in liquid carrier are called ferrofluids or magnetic fluids . A ferrofluid typically has three primary components: ferromagnetic particulates, such as magnetite, and composite ferrite; a surfactant, such as oleic acid or citric acid, and/or tetramethylammonium hydroxide, to Energies 2017, 10, 1025 3 of 21 magnetite, and composite ferrite; a surfactant, such as oleic acid or citric acid, and/or avoid the NPs from clustering, and to a host liquid, suchfrom as mineral oil orand vegetable (as shown in tetramethylammonium hydroxide, avoid the NPs clustering, a hostoil liquid, such as Figure 1). The surfactant is used to coat the particles. This helps in impeding clotting and maintains mineral oil or vegetable oil (as shown in Figure 1). The surfactant is used to coat the particles. This the distribution of particles uniformly throughout the host fluid. Its dispersibility additionally helps in impeding clotting and maintains the distribution of particles uniformly remains throughout the host stable when the magnetic field is applied appropriately [12,20]. One of the elementary necessities fluid. Its dispersibility remains additionally stable when the magnetic field is applied appropriately for a ferrofluid is the stability necessities of magnetic against aggregations. For ferrofluids based on [12,20]. One of the elementary forparticles a ferrofluid is the stability of magnetic particles against dielectric liquids, magneticbased field includes particle cluster exerts significant influence aggregations. Forthe ferrofluids on dielectric liquids, theformation magneticthat field includes particle cluster on the permittivity of the ferrofluid. This phenomenon is called the magnetodielectric effect [9,21,22]. formation that exerts significant influence on the permittivity of the ferrofluid. This phenomenon is The first magnetic colloid with the aim of liquid insulation was produced to improve the heat transfer called the magnetodielectric effect [9,21,22]. The first magnetic colloid with the aim of liquid from the transformer windings by imposing thetransfer magnetic interplay between the field formed by the insulation was produced to improve the heat from the transformer windings by imposing windings and fluid . the magnetic interplay between the field formed by the windings and fluid . Figure 1. Depiction of magnetic nanoparticles (MNPs) in a nanofluid (NF) . Figure 1. Depiction of magnetic nanoparticles (MNPs) in a nanofluid (NF) . The extensive application of MOs for HV insulation and cooling of electrical appliances have extensive application insulationof and cooling of electrical appliances have lead The significant research works of to MOs focus for on HV improvement both its thermal and dielectric features. lead significant research works to focus on improvement of both its thermal and dielectric features. An appropriate creative instance of such a research task is the preparation of dielectric NFs. This An creative instance a research task is the dielectric NFs. This may mayappropriate be achieved by addition of of thesuch MNPs into TO with thepreparation intention ofofimproving the insulating be achieved addition the MNPs into TO with intention of improving theresearch insulating and and thermal by traits [24–26].ofMagnetic nanofluids havethe been the subject of significant due to thermal traits [24–26]. Magnetic nanofluids have been the subject of significant research due to their their particular supermagnetic, tribological, mechanical and thermal features [27–29]. The results particular supermagnetic, tribological, mechanical and thermal [27–29]. The impulse results have have showed that magnetic nanofluids may improve the AC,features DC and lightning (LI) showed that magnetic nanofluids may improve the AC, DC and lightning impulse (LI) breakdown breakdown strength of TO, with certain loadings of Fe3O4 nanoparticles [10,30]. Nevertheless, it was strength TO, withnanoparticles certain loadings Fe3 O4 nanoparticles [10,30]. Nevertheless, was noted noted thatofmagnetic haveof a tendency to agglomerate into larger particles,itparticularly that magnetic nanoparticles havetoaan tendency to agglomerate into larger particles, particularly at at higher concentrations, leading abrupt decease in the breakdown performance of nanofluids higher concentrations, leading to an abrupt decease in the breakdown performance of nanofluids . . Currently, many efforts have been made to raise the dispersion stability of NPs in the host Currently, efforts have been made to raise the dispersion stability NPsnoted in the that hostsurface liquid, liquid, e.g.,many by applying certain dispersants or surfactants [32–36]. It hasofbeen e.g., by applying certain dispersants or surfactants hasthe been noted that surface modified iron oxide NPs show better dispersion [32–36]. stabilityIt in mineral oil by usingmodified various iron oxide NPs show better dispersion stability in the mineral oil by using various synthesizing synthesizing and modifying procedures at room temperature . The dispersion of other NPsand in modifying procedures at room temperature . The dispersion of other NPs in base oil may also be base oil may also be enhanced by tailoring the quantity of modifying agents for surface modification enhanced by tailoring quantity of inherent modifying agents for associated surface modification of nanoparticles of nanoparticles . the To avail these advantages with nanofluids, a number. of To avail these inherent advantages associated with nanofluids, a number of investigation studies have investigation studies have been conducted to formulate the nano-insulation oil. been conducted to formulate the nano-insulation oil. 1.1. Breakdown Phenomenon in Insulating Fluids 1.1. Breakdown Phenomenon in Insulating Fluids One of the most significant parameters of liquid insulation is BDV. The BDV of oils is the value One of the most significant parameters of liquid insulation is BDV. The BDV of oils is the value of of voltage at which the oil is unable to oppose the flow of electricity and that the electricity will go voltage at which the oil is unable to oppose the flow of electricity and that the electricity will go through through it . Molecular ionization of insulating channel, which is dependent on the electric field, it . Molecular ionization of insulating channel, which is dependent on the electric field, is the major is the major phenomenon for electrical breakdown (BD) in TO . After ionization, oil molecules phenomenon for electrical breakdown (BD) in TO . After ionization, oil molecules transform into transform into high mobility electrons and low mobility positive ions, the high speed electrons are high mobility electrons and low mobility positive ions, the high speed electrons are expelled away expelled away to the positive electrode from the ionization channel, because an area of net positive space charge instantly originates. The electric field distribution in the oils is altered during Energies 2017, 10, 1025 4 of 21 to the positive electrode from the ionization channel, because an area of net positive space charge instantly originates. The electric field distribution in the oils is altered during ionization, such that, the electric field ahead of the positive charge in the oil rises, although when it reaches the positive electrode, it tends to decline. The electrodynamics processes motivate an evolving ionizing electric field wave that vaporizes the TO and initiates the gas phase due to the temperature rise. The outcome of oil vaporization is the development of the low density streamer media in the oil . Streamers are edifices having little density that are originated in parts of the oil where the electric field gradient is extreme. 1.2. Ferrofluids in Transformers Mineral oil is mostly applied as a liquid insulating medium in high voltage equipment around the world . Under the electrical stress, the space charge will originate and accumulate within the insulating materials, which may distort the internal electric field distribution and therefore, influence the dielectric breakdown performance [40,41]. A lot of efforts have been made to find the effective ways to decay/suppress the space charge in the insulating materials with an attempt to enhance the dielectric strength and lifetime of insulating materials [42,43]. Recently, nanoparticles with specific electrical and physical characteristics have been applied to boost the insulating properties of TO [24,44]. In recent years, some research investigations on the influence of NPs on the thermal and electrical traits of TO have been conducted. Segal et al.  studied that the suspension of MNPs into MO. They concluded that the AC BDV of the MNFs was improved in comparison to the carrier oil. The positive impulse BDV of ferrofluids showed significant increase, as compared to the base oil, of needle-sphere electrode geometry. The positive and negative LI BDV results of NFs prepared by MNPs conferred by different researchers are compiled in Table 1. Table 1. Results for positive and negative lightning impulse (LI) breakdown voltage (BDV) and time-to-breakdown (BD) for mineral oil (MO) and developed nanofluids. Samples Gap Distance (mm) (+/−) BDV (kV) Time to BD (µs) Streamer Velocity (km/s) Positive Negative Positive Negative Positive Negative Remarks U-60 a U-60-Fe3 O4 nanofluid Nytro b Nytro-Fe3 O4 nanofluid U-60 a U-60-Fe3 O4 nanofluid 25.4/25.4 86 170 12 27 2.12 0.94 25.4/25.4 157 154 26 15 0.98 1.70 25.4/25.4 88 177 16 23 1.58 1.10 25.4/25.4 156 173 25 17 1.016 1.49 55/55 225 340 25 28 2.2 1.96 55/55 390 321 46 32 1.19 1.71 Mineral oil Fe3 O4 nanofluid 5 5 51.84 62.86 83.10 78.54 4.44 5.24 4.02 3.54 1.126 0.954 1.244 1.412 Ref.  Vegetable oil Fe3 O4 nanofluid 15/15 15/15 73.9 101.5 83.8 93.7 9.9 12.0 11.1 12.7 1.51 1.25 1.35 1.18 Ref.  Mineral oil Fe3 O4 nanofluid 3 3 99.1 110.2 - 306 188 - 0.0098 0.0159 - Ref.  a Ref.  Univolt 60 oil, b Nytro 10X oil. In this paper, we intended to enhance the scattering ability of magnetic NPS in the MO at different concentrations. Monodisperse Fe3 O4 NPs modified by oleic acid were produced through solvothermal method. The LI BD strength of the carrier MO and developed magnetic nanofluids with various concentrations of nanoparticles, sizes of nanoparticles and with various electrode gap distance was investigated. Moreover, the probable modification mechanisms of magnetic NPs on dielectric traits of TOs were also reviewed. Energies 2017, 10, 1025 5 of 21 2. Materials and Methods 2.1. Formation of Transformer Oil-Based Ferrofluids (a) Material Selection for Experiment The MNPs (magnetite) are developed in our laboratory. The mineral oil (25#Kelamayi) was processed to remove the impurities and to meet the requisites of pure oil set by CIGRE board 12.17 . As conductive nanoparticles have high surface energy and a tendency to agglomerate, suitable surface modifiers must be chosen to enhance the dispersion characteristics and stability of NPs . Surfactant techniques have been applied to develop a glazed shell on the nanoparticles. The rear ends of surfactant molecules rebuff each other to ensure a distance between the particles to hinder them from agglomeration. Surface modification of NPs is an efficient method to avert NPs agglomeration in insulating liquids [49–52]. Nevertheless, the surface modifiers used for mineral oils cannot be used with other carrier oils, such as vegetable oils, because of different molecular forms/structures. Moreover, some significant features of conductive nanoparticles are also summarized in Table 2. (b) Nanoparticles Synthesis The magnetic nanoparticles Fe3 O4 are developed by applying ferric chloride hexahydrate and iron powder as reactants by a solvo-thermal method. The oleic acid was applied as surface modifiers to ensure uniform distribution of nanoparticles in the mineral oil. In a conventional process, reactants are initially inducted into a combined solution of hexane and dodecylamine under stirring. Post stirring for 5 min, oleic acid was introduced into the aforementioned solution at room temperature with effective agitation. The emerging combination was later heated to the temperature of 180 ◦ C. After heating for 3 h, the derived compound was naturally cooled down, washed with distilled water and absolute ethanol multiple times to eliminate the probable remaining ions in the product, and eventually dried in the vacuum at a temperature of 70 ◦ C . Table 2. Properties of the selected nanoparticles. (c) Properties Transformer Oil Magnetic Nanoparticles (Fe3 O4 ) Conductivity (S/m) [37,54] Relaxation time (s) [37,54] Relative permittivity [37,54] Density (g/cm3 ) Surface modification Material type 10−12 104 –105 7.47 × 10−14 80 5.18 Oleic Acid Conductive 2.2 0.89 Dielectric Development of Nanofluids The typical process was employed to develop transformer oil-based nanofluids with desirable features as follows: (1) (2) (3) (4) The prepared nanoparticles (Fe3 O4 ), after surface modification, are added into MO to the required concentrations, and then ultrasonic processes were applied . The developed nanofluids are acquired and put into vacuum drying for approximately 48 h to exclude the influence of gas bubbles and moisture generated while forming NFs. The moisture content of produced NFs is measured by Rishang coulmetric methods moisture meter JF-5. The flowchart for preparation of nanofluids is shown in Figure 2. The morphology of the prepared NPs is given in Figure 3. The TEM image demonstrates the nano-crystals are uniform and well-distributed without any significant agglomeration. The prepared samples with multiple concentrations are shown in Figure 4. Energies 2017, 10, 1025 Energies 2017, 10, 1025 6 of 21 6 of 21 Energies 2017, 10, 1025 Energies 2017, 10, 1025 6 of 21 6 of 21 Figure 2. Flow chart for nanofluids preparation. Figure 2. Flow chart for nanofluids preparation. Figure 2. Flow chart for nanofluids preparation. Figure 2. Flow chart for nanofluids preparation. Figure 3. TEM image of prepared Fe3O4 nanoparticles (NPs). Figure Figure 3. 3. TEM TEM image image of of prepared prepared Fe Fe33O O44nanoparticles nanoparticles(NPs). (NPs). Figure 3. TEM image of prepared Fe3O4 nanoparticles (NPs). Figure 4. Nanofluids with different nanoparticle concentrations (5% = 0.05 g/L, 10% = 0.1 g/L, 20% = 0.2 g/L, 4. 40% = 0.4 g/L, with 60% different = 0.6 g/L, nanoparticle 80% = 0.8 g/L). Figure Nanofluids concentrations (5% = 0.05 g/L, 10% = 0.1 g/L, 20% = Figure 4. Nanofluids with=different nanoparticle 0.2 g/L, 40% = 0.4 g/L, 60% 0.6 g/L, 80% = 0.8 g/L).concentrations (5% = 0.05 g/L, 10% = 0.1 g/L, 20% = Figure 4. Nanofluids with different nanoparticle concentrations (5% = 0.05 g/L, 10% = 0.1 g/L, 2.2. Electrical Properties of Insulation Fluids 0.2 g/L, 40% = 0.4 g/L, 60% = 0.6 g/L, 80% = 0.8 g/L). 20% = 0.2 g/L, 40% = 0.4 g/L, 60% = 0.6 g/L, 80% = 0.8 g/L). 2.2. Electrical of Insulation All the Properties transformer oils areFluids necessary to fulfill the lightning impulse standards. Many 2.2. Electrical Properties of Insulation Fluids investigations have been conducted by different to measure the breakdown All the transformer oils are necessary to investigators fulfill the lightning impulse standards.voltage Many All the transformer oils are necessary to fulfill the lightning impulse standards.voltage Many and dielectric properties various transformer oilsinvestigators from multiple .breakdown investigations have beenofconducted by different to suppliers measure the investigations have been by different tosuppliers measure the voltage The LI breakdown voltages simulate lightning strikes and normally use. 1.2breakdown microseconds rise and dielectric properties ofconducted various transformer oilsinvestigators from multiple andthe dielectric properties of various transformer oils from multiple suppliers . for wave to reach a magnitude of 90% and then after 50 s, drops to 50% amplitude. The LI The LI breakdown voltages simulate lightning strikes and normally use 1.2 microseconds rise The LI breakdown simulate strikes 1.2amplitude. microseconds for the wave to reach a voltages magnitude of 90%lightning and then after and 50 s,normally drops touse 50% The rise LI for the wave to reach a magnitude of 90% and then after 50 s, drops to 50% amplitude. The LI Energies 2017, 10, 1025 7 of 21 2.2. Electrical Properties of Insulation Fluids All the transformer oils are necessary to fulfill the lightning impulse standards. Many investigations have been conducted by different investigators to measure the breakdown voltage and dielectric properties of various transformer oils from multiple suppliers . The LI breakdown voltages simulate lightning strikes and normally use 1.2 microseconds rise for the wave to reach a magnitude of 90% and then after 50 s, drops to 50% amplitude. The LI breakdown Energies 2017, 10, 1025 7 of 21 voltages are generally measured in accordance with IEC 601897 standard and all the experimentations are executed at room temperature . measured A standard wave is generated by aall tenthe stage breakdown voltages are generally in lightning accordanceimpulse with IEC 601897 standard and generator. An oil vessel with needle to sphere arrangement was employed to measure the breakdown experimentations are executed at room temperature . A standard lightning impulse wave is voltages for formulated exhibited A 25 mmto gap distance was used foremployed positive and generated by a ten NFs stage(as generator. AninoilFigure vessel5). with needle sphere arrangement was measure theLI breakdown voltages forThe formulated (asexposed exhibited Figure 5). A 25voltage mm gap 15 mmtofor negative BDV measurement. samplesNFs were toininitial selected value distance was used for positive and 15 mm for negative LI BDV measurement. The samples were and then were enhanced step by step (2.5 kV in each step) until breakdown takes place. The needle exposed to initialpost selected and then were enhanced conditions. step by step A (2.5 each electrode is changed BD tovoltage ensurevalue the identical experimental setkVofinsix BDstep) voltage until breakdown takes place. The needle electrode is changed post BD to ensure the identical readings were achieved for each sample to enact repeatability. The mean value was considered as LI experimental conditions. A set of six BD voltage readings were achieved for each sample to enact BDV . Whereas, for the legitimacy of the experiments outcomes, three impulse waves must be used repeatability. The mean value was considered as LI BDV . Whereas, for the legitimacy of the at eachexperiments voltage level and each oil sample must endure at least three voltage levels prior the occurrence outcomes, three impulse waves must be used at each voltage level and each oil sample of BD.must endure at least three voltage levels prior the occurrence of BD. Figure 5. Oil tank and electrode geometry. Figure 5. Oil tank and electrode geometry. 3. Results and Discussion 3. Results and Discussion 3.1. Breakdown Strength with Different Concentrations of Nanoparticles 3.1. Breakdown Strength with Different Concentrations of Nanoparticles (a) Positive LI BD Strength of Magnetic Nanofluids (a) Positive BD Strength of Magnetic Nanofluids TheLI positive LI BDV test was conducted for both oil and developed NFs with multiple loadings of NPs. The outcomes are presented in Figure 6. NFs manifested an increase in the LI BDV as The positive LI BDV test was conducted for both oil and developed NFs with multiple loadings of compared to MO. The mean LI BDV strength of NFs was enhanced 36% as compared to carrier TO at NPs. The outcomes are presented in Figure 6. NFs manifested an increase in the LI BDV as compared optimal loading of NPs. It is noted that 40% loading of NPs is the optimum concentration for to MO.positive The mean LI BDV strength was enhanced 36% compared carrier TO at optimal LI BDV. With the riseofinNFs NPs concentration, the as dielectric BDVtoincreases until 40% loading of NPs. It of is NPs. noted that 40% of to NPs is the optimum concentration for positive concentration However, theloading BDV tends decline when the loading of NPs is raised beyond LI BDV. With the rise in NPs concentration, the increases until 40% concentration of NPs. 40% concentration of NPs. The average BDdielectric outcomesBDV of NFs under positive LI BDV with standard deviation are given 3. Inwhen the MNPs loadingsof range 0 and 40%,40% the BDV indicated of However, the BDV tendsintoTable decline the loading NPsbetween is raised beyond concentration an improvement. Beyond the 40% under concentration nanoparticles, the deviation NPs may are start to in NPs. The average BD outcomes of NFs positiveofLIthe BDV with standard given agglomerate and form chains in close proximity of electrodes that give rise to the internal local electric field development and a breakdown initiation at lower voltages . Energies 2017, 10, 1025 8 of 21 Table 3. In the MNPs loadings range between 0 and 40%, the BDV indicated an improvement. Beyond the 40% concentration of the nanoparticles, the NPs may start to agglomerate and form chains in close proximity of electrodes that give rise to the internal local electric field development and a breakdown initiation at10, lower Energies 2017, 1025 voltages . 8 of 21 Energies 2017, 10, 1025 8 of 21 Figure 6. 6. Positive Positive LI LI BDV BDV with with multiple multiple concentrations concentrations (25 mm mm gap distance). distance). Figure Figure 6. Positive LI BDV with multiple concentrations (25 (25 mm gap gap distance). (b) Negative LI BDV Strength of of Magnetic Magnetic Nanofluids Nanofluids (b) (b) Negative LI BDV Strength of Magnetic Nanofluids The negative negativeLI LIBDV BDVmeasurement measurement was conducted oil and various loadings of The was conducted forfor oil and NFsNFs withwith various loadings of NPs. The negative LI BDV measurement was conducted for oil and NFs with various loadings of NPs. The outcomes in Figure 7 indicate that the conductive NPs reduce the negative BD performance The outcomes in Figure 7 indicate that the conductive NPs reduce the negative BD performance of NPs. The outcomes in Figure 7 indicate that the conductive NPs reduce the negative BD performance of MO, which is incompatible with conclusions of others . MO, which is incompatible with thethe conclusions of others . of MO, which is incompatible with the conclusions of others . Figure 7. Negative LI BDV with multiple concentrations (15 mm gap distance). Figure 7. Negative LI BDV with multiple concentrations (15 mm gap distance). Figure 7. Negative LI BDV with multiple concentrations (15 mm gap distance). Table 3. Breakdown outcomes of oil and prepared magnetic nanofluids under LI voltages. Table 3. Breakdown outcomes of oil and prepared magnetic nanofluids under LI voltages. Table 3. Breakdown outcomes of oil and prepared magnetic nanofluids under LI voltages. NPs Loadings (% w/v) Time to BD( µs) Mean Streamer Velocity (km/s) Improvement in BDV (%) NPs Loadings (% w/v) Time to BD( µs) Mean Streamer Velocity (km/s) Improvement in BDV (%) 0 12.87 1.94 0 NPs Loadings Time to BD( µs) Mean Streamer Improvement 0 (% w/v) 12.87 1.94 Velocity (km/s) 0 in BDV (%) 5 14.82 1.68 5.40 50 14.82 1.68 5.40 12.87 1.94 0 10 18.32 1.36 6.21 5 14.82 1.68 5.40 10 18.32 1.36 6.21 20 21.19 1.17 18.38 10 18.32 1.36 6.21 20 21.19 1.17 18.38 20 21.19 1.17 18.38 40 25.33 0.98 36.64 40 25.33 0.98 36.64 40 25.33 0.98 36.64 60 25.08 0.99 29.95 25.08 0.99 29.95 60 25.08 0.99 29.95 80 21.98 1.13 11.40 80 21.98 1.13 11.40 80 21.98 1.13 11.40 3.2. Breakdown Strength with Different Size of Nanoparticles 3.2. Breakdown Strength with Different Size of Nanoparticles (a) Positive LI BDV Strength (a) Positive LI BDV Strength The Positive LI BDV test was tested for oil and developed NFs (with 40% concentrations) with The Positive LI BDV test was tested for oil and developed NFs (with 40% concentrations) with Energies 2017, 10, 1025 9 of 21 3.2. Breakdown Strength with Different Size of Nanoparticles (a) Positive LI BDV Strength The Positive LI BDV test was tested for oil and developed NFs (with 40% concentrations) with various sizes of NPs. The outcomes are indicated in Figure 8. Energies 2017, 10, 1025 of 21 Nanofluids manifested an increase of LI BDV as compared to MO. The mean LI BDV9 of NFs was enhanced, asNanofluids compared to base TO, at optimal size. is significant in the BDV, when Energies 2017, 10, 1025manifested 21 an increase of LI BDVThere as compared to MO.enhancement The mean LI BDV of9 of NFs the size was risesenhanced, from 10 to 20 nm, but a significant reduction is noticed in the BDV, when there is a further as compared to base TO, at optimal size. There is significant enhancement in the manifested ani.e., increase of LIbut BDV as compared to MO. mean NFs BDV,Nanofluids when the size size rises from 10 to40 20nm. nm, aasignificant is The noticed in LI the BDV, when enhancement in the of NPs, As result, it reduction is clear from Figure 3,BDV thatof20 nm is the was enhanced, asenhancement compared toinbase TO, of atNPs, optimal size. There is significant enhancement in the there is a further the size i.e., 40 nm. As a result, it is clear from Figure 3, optimal size of NPs for positive LI BDV. These results are consistent with the previous reportthat [10,31,44]. BDV, size rises 10for to 20 nm, but significant reduction noticed in the the BDV, when 20 nmwhen is thethe optimal size from of NPs positive LI aBDV. These results are is consistent with previous It is concluded that the increase of nanoparticle size will weaken the modification effect on breakdown there a further enhancement in the NPs, i.e., nm. As a result, it isweaken clear from 3, that reportis[10,31,44]. It is concluded thatsize the of increase of 40 nanoparticle size will theFigure modification strength20 of nanofluids. nm is the optimal size of NPs for positive LI BDV. These results are consistent with the previous effect on breakdown strength of nanofluids. report [10,31,44]. It is concluded that the increase of nanoparticle size will weaken the modification effect on breakdown strength of nanofluids. Figure 8. The effect of size on positive LI BDV (gap distance 25 mm). Figure 8. The effect of size on positive LI BDV (gap distance 25 mm). Figure 8. The effect of size on positive LI BDV (gap distance 25 mm). (b) Negative LI Breakdown Strength (b) Negative LI Breakdown Strength Negative LI LI Breakdown BDV measurement (b) Negative Strengthwas conducted for both MO and NFs. The outcomes are shown in FigureLI9.BDV The negative LI BDV decreases with the rise of sizeMO of NPs. negative LI BDVs of are the shown Negative measurement was conducted for both andThe NFs. The outcomes Negative LI BDV measurement was conducted for both MO andoil, NFs. The outcomes are shown prepared NFs with various sizes of NPs are lower than that of pure which is incompatible with in Figure 9. The9.negative LI BDV decreases with the rise of size of NPs. The negative LI BDVs of the in The negative theFigure results of others . LI BDV decreases with the rise of size of NPs. The negative LI BDVs of the prepared NFs with various sizessizes of NPs areare lower oil,which which incompatible prepared NFs with various of NPs lowerthan thanthat that of of pure pure oil, is is incompatible withwith the results the of others . results of others . Figure 9. The influence of size on negative LI BDV (gap distance 15 mm). Figure 9. The influence of size on negative LI BDV (gap distance 15 mm). Figure 9. The influence of size on negative LI BDV (gap distance 15 mm). Energies 2017, 10, 1025 Energies Energies2017, 2017,10, 10,1025 1025 10 of 21 10 10ofof21 21 3.3. 3.3. Breakdown Strength with Different Gap Distance 3.3.Breakdown BreakdownStrength Strengthwith withDifferent DifferentGap GapDistance Distance (a) (a) Positive LI BDV Strength (a) Positive PositiveLI LIBDV BDVStrength Strength Positive MO and developed NFs (with 40% loadings and 20 PositiveLI testwas was conducted for both MO and developed NFs (with 40% loadings and 20 Positive LIBDV BDVtest wasconducted conductedfor forboth both MO and developed NFs (with 40% loadings and nm size) with different gap distances. The outcomes are nmnm size) with different gap distances. The outcomes are given in Figure 10.Nanofluids Nanofluidspointed pointedout out 20 size) with different gap distances. The outcomes aregiven givenin inFigure Figure10. pointed out an anenhancement enhancementof ofLI LIBDV BDVthan thanMO MOfor forall allgap gapdistances. distances.The TheBDVs BDVsfor forall allNFs NFssamples samplesimproves improves an enhancement of LI BDV than MO for all gap distances. The BDVs for all NFs samples improves with the increase of the gap distance. The result attained from this study is agreeable with the withthe theincrease increaseof ofthe thegap gapdistance. distance. The The result result attained attained from from this this study study is is agreeable agreeable with with the theresults results with results of ofother otherresearchers researchers[58,59]. [58,59].BDVs BDVsof ofNFs NFsare arealways alwayshigher higherthan thanMO MOfor forall allgap gapdistances. distances. of other researchers [58,59]. BDVs of NFs are always higher Figure Figure 10. Positiveimpulse impulsebreakdown breakdown strength with different needle to sphere gap distances. Figure10. 10.Positive breakdownstrength strengthwith withdifferent differentneedle needleto tosphere spheregap gapdistances. distances. (b) Negative LI BDV Strength (b) (b) Negative NegativeLI LIBDV BDVStrength Strength Negative LI BDV measurement was done for both MO and nanofluids at different needle to Negative NegativeLI LIBDV BDVmeasurement measurementwas wasdone donefor forboth bothMO MOand andnanofluids nanofluidsat atdifferent differentneedle needleto to sphere gap distances. The results are indicated in Figure 11. The results are inconsistent with the sphere spheregap gapdistances. distances.The Theresults resultsare areindicated indicatedin inFigure Figure11. 11.The Theresults resultsare areinconsistent inconsistentwith withthe the conclusions of others . The negative LI BDVs for NFs are always lower than that of MO for all conclusions conclusionsof ofothers others. .The Thenegative negativeLI LIBDVs BDVsfor forNFs NFsare arealways alwayslower lowerthan thanthat thatof ofMO MOfor forall all investigated electrode gap distances. investigated electrode gap distances. investigated electrode gap distances. Figure Figure11. 11.Negative Negativeimpulse impulsebreakdown breakdownstrength strengthwith withdifferent differentneedle needletotosphere spheregap gapdistances. distances. Figure 11. Negative impulse breakdown strength with different needle to sphere gap distances. 3.4. 3.4.Breakdown BreakdownMechanism Mechanism Energies 2017, 10, 1025 11 of 21 3.4. Breakdown Mechanism The investigations further elaborated on the concept that the space charges effect in TO is a significant determinant that affects the inception and origination of streamer discharge . The insulation BD strength of TOs is closely linked to the electric field and its internal space charge [55,61–63]. Many researchers suppose that the distinctive interface features between oil and nanoparticles perform an imperative role in the space charge transport during the BD mechanism in NFs [64–66]. The interface area comprise of enormous sum of electronic traps that can abduct and deliver electrons frequently. The process of trapping and de-trapping decreases the velocity and energy transfer of electrons and obstructs the further evolution of the streamer. Other researchers  believe that suspended nanoparticles introduce additional traps, which can capture the electrons and reduce the average energy of electrons travelling through the oil, and so the possibility of further electron production through impact ionization is also decreased. Therefore, the distortion of electric field in the oil by the electronic charge in transit would be decreased, and then hence, the dielectric strength is improved. The BD process of TO stressed by applied voltages is largely associated with the electric field and space charge distribution in TO. The decrease of space charge density and uniform electric field in transformer oil can upgrade the breakdown voltage of the TO. It is believed that the introduction of Fe3 O4 NPs into TO behaves as electron scavengers and captures electrons, transforming them into slow charged nanoparticles in the nanofluids. This conduct reduces the space charge density and result in a more uniform electric field distribution. Streamer development in the nanofluids is inhibited, and the BD performance of nanofluids is improved. (a) Mechanism of Action of Magnetic Nanoparticles From the conventional point of view, the existence of conductive particles into MO may act as impurity and must reduce its dielectric performance, but the experiments have manifested that distribution of conductive NPs into MO have demonstrated an improvement in its breakdown performance. Therefore, it is useful and essential to comprehend what makes the NFs have distinct BD features, as compared to carrier oil for new oil-paper insulation systems with favorable dielectric characteristics. The charge relaxation time constant of NP materials is deliberated to perform a dominant role in the electrodynamics processes in transformer oil. If the charge relaxation time constant of nanoparticles is shorter relative to time scales of interest for streamer development; their existence in the oil will effectively alter the electrodynamics. If, on the other hand, the nanoparticles’ charge relaxation time constant is relative to the time scales of interest for streamer expansion, their existence will have minor effect on the electrodynamics . The charge relaxation constant (τ r ) for mineral oil/nanoparticle is: 2ε + ε 2 τr = 1 2σ1 + σ2 where ε1 , σ1 , ε2 , and σ2 are permittivity and electrical conductivity of mineral oil and nanoparticle, respectively. A smaller value of relaxation time constant means faster electron absorption of nanoparticles. According to the authors of , the relaxation time constant of conductive MNPs (7.47 × 10−14 s) is less than the nanosecond to microsecond of propagation time of the streamer. The surface of the magnetic nanoparticles (Fe3 O4 ) may consume the free electrons and hence, alter the potential distribution around the particle . Therefore, the suspension of MNPs into transformer oil may effectively influence the electrodynamics process during the streamer development, and ultimately, enhance the BD performance of magnetite NFs. Energies 2017, 10, 1025 (b) 12 of 21 Analysis of Mechanism Improved Breakdown Properties It is considered that the modifications in space charge distributions are motivated by the 12 of 21 suspension of nanoparticles into MO and therefore, the breakdown features of nanofluids and pure oil are different. This work explicates thebetween foregoing conditions by applying the needle–sphere model. in The rising positive LI voltages electrodes originate a corona discharge to happen The rising positive LI voltages between electrodes originate a corona discharge to happen in close proximity to the positive needle electrode with high local electric field strength. This high local close proximity to the positive needle electrode with high local electric field strength. This high local electric field strength causes ionization of molecules in the transformer oil, close to the needle electric field causes ionization the transformer close to the needle electrode. electrode. A strength significant space charge of is molecules developedindue to this fieldoil, ionization. The electrons are A significant space charge is developed due to this field ionization. The electrons are produced at a produced at a high electric field and are neutralized at the needle electrode in pure oil. After electron high electric field neutralized at thethere needleare electrode in pure oil. After electron neutralization neutralization at and the are needle electrode, a significant number of positive ions left at the needle electrode, there are a significant number of positive ions left accumulated close the accumulated close to the needle electrode due to relatively low mobility of these particles.toThis needle electrode due to relatively low mobility of these particles. This newly developed spatial electric newly developed spatial electric field undermines the external field close to the needle electrode and field undermines the external field close to the ions needle electrode and invigorates the external field invigorates the external field between positive and sphere electrode. This developed spatial between positive ions and sphere electrode. This developed spatial electric field causes the strong electric field causes the strong distortion effect responsible for an early electric breakdown in pure distortion effect 12). responsible for an early electric breakdown in pure oil (as in Figure 12). oil (as in Figure In case caseof ofNFs, NFs,some someportion portion high mobility electrons generated molecular ionization In of of high mobility electrons generated afterafter molecular ionization due due to high local electric field stress is neutralized after approaching the needle electrode, whereas to high local electric field stress is neutralized after approaching the needle electrode, whereas the the remaining segment of electrons is abducted by suspended nanoparticles in Figure 13). remaining segment of electrons is abducted by suspended nanoparticles (as in(as Figure 13). The The nanoparticles are transformed negative ions after abduction electrons.As Asthe themobility mobility of of nanoparticles are transformed intointo negative ions after abduction ofofelectrons. these negative ions developed is low, a large number of these negatively charged NPs are left in the these negative ions developed is low, a large number of these negatively charged NPs are left in the ionization zone zone close close to to the the needle needle electrode. electrode. This This mal-position mal-position of of positive positive and and negative negative ions ions close close to to ionization the needle electrode results in a superposition spatial electric field, which distorts the former electric the needle electrode results in a superposition spatial electric field, which distorts the former electric field. The The existence existence of of these these negatively negatively charged charged NPs NPs close close to to the the needle needle electrode electrode abate abate the the distortion distortion field. effect responsible responsible for for an an early early breakdown breakdown in in pure pure oil. effect oil. Energies 2017, 10, 1025 Figure 12. Space charge build-up under positive impulse voltage in transformer oil. Figure 12. Space charge build-up under positive impulse voltage in transformer oil. The corona discharge developed in nanofluids is harder to expand outwards than the corona discharge in pure oil when the voltages are enhanced continuously. The positive charges move toward sphere electrode and negatively charged nanoparticles moves towards the needle electrode. In this way, the distortion effect of the space charge field on the prior field is less than in the pure oil. Thus, the positive LI breakdown voltages are improved after the distribution of nanoparticles. nanoparticles will capture the electrons generated after molecular ionization and transformed into negatively charged particles. A large number of negatively charged NPs will remain close to the needle electrode due to their low mobility. This phenomenon undermines the electric filed strength near the needle and bolsters the electric field near the sphere electrode. Thus, the breakdown 2017, 10, 1025 13 of 21 happensEnergies at lower negative voltages for nanofluid as compared to the pure oil (Figure 14). FigureFigure 13. Space charge build-up positive impulse voltage in nanofluids. 13. Space charge build-upunder under positive impulse voltage in nanofluids. The corona discharge developed in nanofluids is harder to expand outwards than the corona discharge in pure oil when the voltages are enhanced continuously. The positive charges move toward sphere electrode and negatively charged nanoparticles moves towards the needle electrode. In this way, the distortion effect of the space charge field on the prior field is less than in the pure oil. Thus, the positive LI breakdown voltages are improved after the distribution of nanoparticles. On the contrary, the condition under negative LI voltage is quite contrasting. In pure oil, after the application of negative impulse voltages to the needle electrode, the molecular ionization occurs close to the needle electrode after corona generation and the space charges are developed. The ionization of molecules will produce high mobility electrons, which will tend to move towards the sphere electrode and leave behind the positive ions close to the needle electrode. A portion of these positive ions is neutralized after approaching the needle electrode and the remaining part will retain near the needle electrode due to the low mobility of the positive ions. In case of nanofluids, the nanoparticles will capture the electrons generated after molecular ionization and transformed into negatively charged particles. A large number of negatively charged NPs will remain close to the needle electrode due to their low mobility. This phenomenon undermines the electric filed strength near the needle and bolsters the electric field near the sphere electrode. Thus, the breakdown happens at lower negative voltages for nanofluid as compared to the pure oil (Figure 14). EnergiesFigure 2017, 10, 1025 13. Space charge build-up under positive impulse voltage in nanofluids. 14 of 21 Energies 2017, 10, 1025 14 of 21 14. Space charge build-upunder under negative lightning impulse voltage. FigureFigure 14. Space charge build-up negative lightning impulse voltage. 4. Research Challenges, Technical Difficulties, and Gaps 4. Research Challenges, Technical Difficulties, andResearch Research Gaps Although the transformer oil-based ferrofluids have manifested excellent dielectric and thermal Although the transformer oil-based ferrofluids have manifested excellent dielectric and thermal properties and are considered as potential substitute of mineral oils to be applied in high voltage properties and are as potential substitute mineral to be applied in high equipment in considered the years to come, but the challenges whichof restrain theiroils applications still persists. Also, voltage equipment years issues to come, but the challenges which restrain their applications still persists. thereinarethe numerous and other challenges that need to be further examined. There are challenges and problems associated with ferrofluids research that, we think, are closely linked to each other. Also, there are numerous issues and other challenges that need to be further examined. There are challenges problems 4.1. and Research Challengesassociated with ferrofluids research that, we think, are closely linked to each other. The features of ferrofluids depend on the variety of factors including, method of preparation, type of base oil, and combinational characteristics of nanoparticles and oil. 4.1. Research Challenges (a) Synthesis of Ferrofluids The features of ferrofluids depend on the variety of factors including, method of preparation, use of nanoparticles mainly depends upon the synthesis method/process of NFs. type of base The oil, successful and combinational characteristics of nanoparticles and oil. Particular requirements, such as stable suspension, controlled size and concentration of nanoparticles are necessary. Normally, there are two methods of development of nanofuids: single-step and (a) Synthesis of Ferrofluids two-step method. Each method has its advantages and disadvantages. The one-step method is for developing nanofluids which consists of high conductive metals tomethod/process hinder oxidation. of NFs. Thefavorable successful use of nanoparticles mainly depends upon the synthesis The disadvantage of the single step technique is its limited control over significant factors such as size Particular requirements, such as stable suspension, controlled size and concentration of of nanoparticle. Preparing nanofluids by using two-step technique is also very challenging, because of nanoparticles are necessary. Normally, there are two methods of development of nanofuids: potential agglomeration of nanoparticles. The issue of agglomeration becomes very serious at higher single-step andconcentrations. two-step method. Each method has its advantages and disadvantages. The one-step volume method is favorable for developing nanofluids which consists of high conductive metals to hinder oxidation. The disadvantage of the single step technique is its limited control over significant factors such as size of nanoparticle. Preparing nanofluids by using two-step technique is also very challenging, because of potential agglomeration of nanoparticles. The issue of agglomeration becomes very serious at higher volume concentrations. Energies 2017, 10, 1025 (b) 15 of 21 Stability of Ferrofluids The tendency of nanoparticles to merge into larger particulates under attractive forces and external stresses can adhere together and produce aggregates of larger size, which may settle out of suspension because of gravity [68,69]. Agglomeration means that the particles begin to aggregate at a meaningful rate. The agglomeration is one of the most important issues for a (liquid-solid) two-phase system. The agglomeration of nanoparticles may act as a weak link, from which a disastrous process usually initiates, leading to deterioration of not only dielectric properties, but also thermal characteristics of liquid insulation. For instance, the electrical breakdown performance of transformer oil suspended with conductive nanoparticles was found to be adversely influenced by the presence of significant agglomerates of nanoparticles . Thermal conductivity of liquid insulation is also affected by nanoparticles agglomeration . Therefore, the suitable addition of nanoparticles into transformer oil needs to be accomplished to ensure the optimized properties of the resulting ferrofluids. The agglomeration of magnetic nanoparticles may be reduced by the use of certain surfactants, surface modification techniques and ultrasonic agitation [72–75]. (c) Application of Surfactants and Surface Modification Although the use of surfactants and surface modification of NPs has illustrated a potential to enhance the dispersion stability of magnetic nanoparticles at low concentrations, but the stability of magnetic nanofluids with higher concentrations is still a significant challenge. The inclusion of surfactants decreases the surface tension of base fluids and enhances the immersion of NPs. Dispersants or surfactants are chemical compounds applied to NPs in order to reduce the surface tension of fluids and enhance the immersion of nanoparticles. The excess of surfactant may also cause instability. The excess of surfactant will dissociate from the surface of nanoparticles and may dissolve into the mineral oil as an impurity, thus adversely affecting the breakdown strength on NFs. The addition of surfactants in the two-phase systems is an easy and economic technique to improve the stability of NFs. The selection of suitable dispersants is also a major challenge. The surface modification technique is a surfactant-free approach and it uses functionalized nanoparticles to attain a long-term stability of nanofluids. This technique is applied to enhance the dispersion of NPs and to improve the compatibility between NPs and liquid materials. (d) Dielectric Improvement Mechanism The mechanism of dielectric enhancement of breakdown properties of transformer oil is not fully elaborated. Hwang et al.  presented the electron scavenging model which is dependent on the relaxation time constant. It may describe the enhancement of insulating strength of oil with conductive (Fe3 O4 ) NPs distribution, but it is incapable of explaining the insulating strength improvement of other conductive, semiconductive and insulative nanoparticles suspensions. For instance, Chiesa et al.  manifested that other type of conductive nanoparticles (σ = 1 × 102 S/m) with a short relaxation time constant (τ = 1.1 × 10−12 s) is unable to enhance BD strength of TO. The electron scavenging by conductive nanoparticles deduced by the relaxation time constant, which was not able to describe this phenomenon. Thus, it is also a significant challenge in nanofluids research to explore the modification mechanism of NPs on dielectric characteristics of TO. (e) Other Related Issues and Challenges The investigations have manifested that the electrical conductivity, relative permittivity and loss factor of prepared magnetic fluids is very different from the host oil . The practical application of magnetic fluids in transformers with these unique properties may have different electrical stress distribution and thus have severe complications on the transformer structure. The standard maintenance and testing procedures also need to be revised. The long term oxidation stability of Energies 2017, 10, 1025 16 of 21 magnetic fluids also needs to be improved, and other related issues also still need to be investigated, such as sedimentation problems, oxidation stability, as well as moisture absorption. 4.2. Technical Problems and Difficulties The major technical difficulties regarding the use of magnetic fluids as insulation and cooling liquid in high voltage equipment, which require further investigations, are summarized as below [44,77]: (1) (2) (3) (4) It is complicated to apply magnetic fluids in the existent transformers because of disparity of the electrical specifications, so it is necessary to conduct more research work regarding the application of magnetic fluids in these existing transformers. More investigative studies are needed to explore more efficient synthesis processes, to decrease the production cost of FFs and to recognize the potential industrial applications of ferrofluids. A significant research is necessary to curtail the severe human body and environmental impacts of transformer oil-based ferrofluids. The coating chemistry of nanoparticles have a significant influence on the dielectric features of a ferrofluid, therefore more research work is required to discover a better coating chemistry for magnetic nanoparticles. 4.3. Other Problems and Research Gap Although transformer oil-based ferrofluids have demonstrated exceptionally interesting dielectric properties, but still there are some imperative issues and challenges which require attention. The following crucial problems must be given thorough focus in subsequent research work. Firstly, more experimental and theoretical investigations are required to explain the mechanism of enhancement of dielectric BD strength of ferrofluids. Secondly, up to now, there is an inadequacy of agreement between the experimental results obtained by various researchers, so it is important to conduct more research about the precise and definite development of ferrofluids and it may be significant to elaborate the discrepancy between experimental results. Thirdly, the agglomeration of nanoparticles is a very critical problem, from both a research perspective and a view of practical applications. This issue can be reduced to a certain extent by the application of surface modifiers on nanoparticles, but still more research work is necessary for the long term stability of ferrofluids. Lastly, the size and shape of magnetic nanoparticles are crucial for characterization of ferrofluids; thus, a modern synthesis approach will also make for interesting research inquiry in the near future. 5. Advantages and Disadvantages of Transformer Oil-Based Ferrofluids 5.1. Advantages of Transformer Oil-Based Ferrofluids The transformer oil-based ferrofluids possess many performance advantages as compared to transformer oils and are summarized as follows [9–13,21–24,30–33,40–44]: (i) The transformer oil-based ferrofluids have better AC and impulse breakdown performance as compared to mineral oils, so it is favorable to be used in high voltage alternating current (HVAC) and high voltage direct current (HVDC) applications. (ii) The AC BD strength of transformer oil-based ferrofluids is less influenced by moisture as compared to mineral oils, so it is helpful in improving insulation life of transformers. (iii) The transformer oil-based ferrofluids have better partial discharge characteristics, as compared to mineral oil. (iv) The transformer oil-based ferrofluids have a better anti-aging characteristic, as compared to MO, so it can improve the operational reliability and lifetime of high voltage transformers. (v) The transformer oil-based ferrofluids have a higher thermal conductivity than the transformer oil and they are more helpful in cooling the transformers. Energies 2017, 10, 1025 17 of 21 5.2. Disadvantages of Transformer Oil-Based Ferrofluids The use of ferrofluids provides a better breakdown performance, partial discharge characteristics, and anti-aging properties than transformer oil , but there still are some parameters which limit their use on a large scale in industrial and commercial applications. The application of ferrofluids in industrial application requires long-term stability, low cost availability, and understanding of the brunt of nanomaterials on human health and environment. In this section, an overview of stability of ferrofluids and their impact on human health and the environment is presented [9–13,21–24,30–33,40–44]. (a) Agglomeration of Particles A ferrofluids is known as theoretically stable if the particle size is smaller than 100 nm . However, it is a big challenge to keep this size due to existence of attractive forces between nanoparticles, which can lead to the agglomeration of nanoparticles. The sedimentation arises in most of the ferrofluids, due to gravity, and the fact that the density of nanoparticles is higher than that of mineral oil, which could lead to a reduction in breakdown voltages. (b) Human Health Problems Nanoparticles have been considered as one of the major health and safety hazards for human body. Nanoparticles have been recognized as more dangerous than the micron-sized or bulk materials, due to the high reactivity of their surface area . One way of infiltration of nanoparticles into the human body may be through the nasal cavity [79,80]. The exposure of smaller quantity of nanoparticles is even more vulnerable to the health. For instance, iron oxide is recognized more detrimental for human lungs [81,82]. The nanoparticles, if they invade through the digestive system, may invade the blood stream and accumulate in the liver . The required safety measures should be taken while preparing ferrofluids to abstain from the above mentioned risks. (c) Higher Cost of Ferrofluids The higher development cost of ferrofluids is one the reasons hindering their application on commercial and industrial levels. The preparation of magnetite nanoparticles methods and development processes of ferrofluids make them expensive substitutes of transformer oils. 6. Conclusions In this work, the dielectric strength of transformer oil with and without the suspension of MNPs with different concentrations and sizes of nanoparticles was measured. Moreover, the positive LI BD strength was also measured with different electrode gap distances of needle to sphere geometry. The results manifested the improvement in the breakdown strength of transformer oil after the addition of MNPs into it. Results of positive impulse BDV at various concentrations revealed that at 40% concentration of NPs, the mean LI BDV was 1.36 times as compared to carrier oil and 40% concentration was recognized as the optimum concentration. Volume concentration above this value tends to reduce in positive LI BDV. Results of positive impulse breakdown voltages at different sizes revealed that at 20 nm size of nanoparticles, the mean lighting impulse breakdown voltages were maximum as compared to base oil and that 20 nm is the optimum size of nanoparticles in this study. The results of negative LI BDV of magnetic fluids with various concentrations and sizes were lower than that of the BD strength of host MO. The lightning impulse breakdown voltages at different electrode distances were also measured. It is concluded that the transformer oil suspended with magnetic nanoparticles has manifested good dielectric characteristics; therefore, it may be a good substitute to mineral oil, with suitable volume concentration and size of nanoparticles, in the future. Energies 2017, 10, 1025 18 of 21 Acknowledgments: The authors would like to express gratitude to National Natural Science Foundation of China for aiding this study under Contract Nos. 51337003, 51472084, and 51477052 and the Fundamental Research Funds for the Central Universities (JB2015019). Author Contributions: The experiments were guided by Yuzhen Lv. Muhammad Rafiq and Bingliang Shan characterized the nanofluids. Chengrong Li and Yuzhen Lv participated in the discussion and gave valuable suggestions. The manuscript was composed by Muhammad Rafiq. All authors approved the final manuscript. Conflicts of Interest: The authors acknowledge that there is no conflict of interests regarding the publication of this article. References 1. 2. 3. 4. 5. 6. 7. 8. 9. 10. 11. 12. 13. 14. 15. 16. 17. 18. 19. 20. 21. Rafiq, M.; Lv, Y.Z.; Zhou, Y.; Ma, K.B.; Wang, W.; Li, C.R.; Wang, Q. Use of vegetable oils as transformer oils—A review. Renew. Sustain. Energy Rev. 2015, 52, 308–324. [CrossRef] Peterchuck, D.; Pahwa, A. Sensitivity of transformer’s hottest-spot and equivalent aging to selected parameters. IEEE Trans. Power Deliv. 2002, 17, 996–1001. [CrossRef] Bartley, W.H. Investigating transformer failure. In Proceedings of the Weidmann-ACTI 5th Annual Technical Conference on New Diagnostic Concepts for Better Asset Management, Albuquerque, NM, USA, 13–15 November 2006. EPRI Portfolio 2007—Transmission Reliability and Performance: 37.002, Transformer Life Extension. Available online: http://www.epri.com/portfolio/ (accessed on 17 May 2016). Chiesa, M.; Das, S.K. Experimental investigation of the dielectric and cooling performance of colloidal suspensions in insulating media. Coll. Surf. A Physicochem. Eng. Asp. 2009, 335, 88–97. [CrossRef] Rouse, T.O. Mineral insulating oil in transformers. IEEE Electr. Insul. Mag. 1998, 14, 6–16. [CrossRef] Lundgaard, L.E.; Hansen, W.; Linhjell, D.; Painter, T.J. Aging of oil-impregnated paper in power transformers. IEEE Trans. Power Deliv. 2004, 19, 230–239. [CrossRef] Rafiq, M.; Lv, Y.Z.; Li, C.R. A Review on Properties, Opportunities, and Challenges of Transformer Oil-Based Nanofluids. J. Nanomater. 2016, 2016. [CrossRef] Segal, M.V.; Raj, K. An investigation of Power Transformer Cooling with magnetic Fluid. Indian J. Eng. Mater. Sci. 1998, 5, 416–422. Kopcansky, P.; Tomco, L.; Marton, K.; Koneracka, M.; Timko, M.; Potocova, I. The DC dielectric breakdown strength of magnetic fluids based on transformer oil. J. Magn. Magn. Mater. 2005, 289, 415–418. [CrossRef] Erdman, H.G. Electrical Insulating Oils STP 998; ASTM Publ. Co.: Philadelphia, PA, USA, 1996. Choi, S. Enhancing Thermal Conductivity of Fluids with Nanoparticles. In Proceedings of the ASME International Mechanical Engineering Congress & Exposition, San Francisco, CA, USA, 12–17 November 1995; Volume 231, p. 99. Rosensweig, R.E. Ferrohydrodynamics; Cambridge Univeersity Press: Cambridge, UK, 1985; p. 7. Das, S.K.; Choi, S.; Yu, W.; Pradeep, T. Nanofluids: Science and Technology; John Wiley & Sons, Inc.: Madras, Indian, 2008; p. 5. Khurshid, H.; Nemati, J.A.Z.; Phan, M.H.; Mukherjee, P.; Fdez-Gubieda, M.L.; Barandiaran, J.M.; Srikanth, H. Anisotropy effects in magnetic hyperthermia: A comparison between spherical and cubic exchange-coupled FeO/Fe3 O4 nanoparticles. J. Appl. Phys. 2015, 117, 17A337. [CrossRef] Parchur, A.K.; Ansari, A.A.; Singh, B.P.; Hasan, T.N.; Syed, N.A.; Rai, S.B.; Ningthoujam, R.S. Ultrafast vibrational dynamics and spectroscopy of a siloxane self-assembled monolayer. J. Chem. Phys. 2011, 134, 084701. Wu, Z.S.; Yang, S.; Sun, Y.; Parvez, K.; Feng, X.; Mullen, K. Nitrogen-doped graphene aerogel-supported Fe3 O4 nanoparticles as efficient electrocatalysts for the oxygen reduction reaction. J. Am. Chem. Soc. 2012, 134, 9082. [CrossRef] [PubMed] He, H.; Gao, C. Supraparamagnetic, conductive, and processable multifunctional graphene nanosheets coated with high-density Fe3 O4 nanoparticles. ACS Appl. Mater. Interface 2010, 2, 3201. [CrossRef] [PubMed] Nkurikiyimfura, I.; Wang, Y.; Pan, Z. Heat transfer enhancement by magnetic nanofluids—A review. Renew. Sustain. Energy Rev. 2013, 21, 548–561. [CrossRef] Odenbach, S. Magnetoviscous Effects in Ferrofluids; Springer: Berlin, Germany, 2002. Ayoub, N.Y.; Bradbury, A.; Chantrell, R.W.; Popplewell, J. A ‘pair orientation’ model of the magnetodielectric anisotropy in ferrofluids. J. Magn. Magn. Mater. 1987, 65, 185. [CrossRef] Energies 2017, 10, 1025 22. 23. 24. 25. 26. 27. 28. 29. 30. 31. 32. 33. 34. 35. 36. 37. 38. 39. 40. 41. 42. 43. 19 of 21 Kopcansky, P.; Cernak, J.; Macko, P.; Spisak, D.; Marton, K. Dielectric behaviour of mineral-oil-based magnetic fluids-the cluster model. J. Phys. Appl. Phys. 1989, 22, 1410–1412. [CrossRef] Yusuf, N.A.; Shobaki, J.; Abu-Safia, H.; Abu-Aljarayesh, I. Magneto-dielectric anisotropy in magnetic fluids determined from magneto-optical measurements. J. Magn. Magn. Mater. 1995, 149, 373. [CrossRef] Segal, V.; Rabinovich, A.; Nattrass, D.; Raj, K.; Nunes, A. Experimental study of magnetic colloidal fluids behavior in power transformers. J. Magn. Magn. Mater. 2000, 513, 215–216. [CrossRef] Segal, V.; Nattrass, D.; Raj, K.; Leonard, D. Accelerated thermal aging of petroleum-based ferrofluids. J. Magn. Magn. Mater. 1999, 70, 201. [CrossRef] Segal, V.; Hjortsberg, A.; Rabinovich, A.; Nattrass, D.; Raj, K. AC (60 Hz) and impulse breakdown strength of a colloidal fluid based on transformer oil and magnetite nanoparticles. In Proceedings of the Conference Record of the 1998 IEEE International Symposium on Electrical Insulation, Arlington, VA, USA, 7–10 June 1998; pp. 619–622. Philip, J.; Shima, P.D.; Raj, B. Enhancement of thermal conductivity in magnetite based nanofluid due to chainlike structures. Appl. Phys. Lett. 2007, 91, 203108. [CrossRef] Cha, H.G.; Kim, C.W.; Kang, S.W.; Kim, B.K.; Kang, Y.S. Preparation and characterization of the magnetic fluid of trimethoxyhexadecylsilane-coated Fe3 O4 nanoparticles. J. Phys. Chem. 2010, 114, 9802–9807. Sharifi, I.; Shokrollahi, H.; Amiri, S. Ferrite-based magnetic nanofluids used in hyperthermia applications. J. Magn. Magen. Mater. 2012, 324, 903–915. [CrossRef] Sima, W.X.; Cao, X.F.; Yang, Q. Preparation of three transformer oil-based nanofluids and comparison of their impulse breakdown characteristics. Nanosci. Nanotechnol. Lett. 2014, 6, 250–256. [CrossRef] Lee, J.C.; Lee, W.H.; Lee, S.H.; Lee, S. Positive and negative effects of dielectric breakdown in transformer oil based magnetic fluids. Mater. Res. Bull. 2012, 47, 2984–2987. [CrossRef] Viali, W.R.; Alcantara, G.B.; Sartoratto, P.P.C.; Soler, M.A.G.; Mosiniewiczszablewska, E.; Andrzejewski, B. Investigation of the molecular surface coating on the stability of insulating magnetic oils. J. Phys. Chem. C 2010, 114, 179–188. [CrossRef] Lu, Y.Z.; Zhang, S.N.; Du, Y.F.; Chen, M.T.; Li, C.R. Effect of Oleic Acid Surface Modification on Dispersibility of TiO2 Nanoparticles in Transformer Oils. J. Inorg. Mater. 2013, 28, 594–598. [CrossRef] Thorat, N.D.; Khot, V.M.; Salunkhe, A.B.; Prasad, A.I.; Ningthoujam, R.S.; Pawar, S.H. Surface functionalized lsmo nanoparticles with improved colloidal stability for hyperthermia applications. J. Phys. D Appl. Phys. 2013, 46, 105003–105013. [CrossRef] Veriansyah, B.; Chun, M.S.; Kim, J. Surface-modified cerium oxide nanoparticles synthesized continuously in supercritical methanol: Study of dispersion stability in ethylene glycol medium. Chem. Eng. J. 2011, 168, 1346–1351. [CrossRef] Zhou, J.; Song, B.; Zhao, G.; Han, G. Effects of acid on the microstructures and properties of three-dimensional TiO2 , hierarchical structures by solvothermal method. Nanoscale Res. Lett. 2012, 7, 1–10. [CrossRef] [PubMed] Du, Y.F.; Lv, Y.Z.; Wang, F.C.; Li, X.X.; Li, C.R. Effect of TiO2 nanoparticles on the breakdown strength of transformer oil. In Proceedings of the Conference Record of the 2010 IEEE International Symposium on Electrical Insulation (ISEI’10), San Diego, CA, USA, 6–9 June 2010; pp. 1–3. O’Sullivan, F.; Hwang, J.G.; Zahn, M.; Hjortstam, O.; Pettersson, L.; Liu, R.; Biller, P. A model for the initiation and propagation of positive streamers in transformer oil. In Proceedings of the IEEE International Symposium on Electrical Insulation (ISEI’08), Vancouver, BC, Canada, 9–12 June 2008; pp. 210–214. Hwang, J.G.; Zahn, M.; O’Sullivan, F.M.; Pettersson, L.A.A.; Hjortstam, O.; Liu, R. Electron scavenging by conductive nanoparticles in oil insulated power transformers. In Proceedings of the Electrostatics Joint Conference, Boston, MA, USA, 16–18 June 2009. Blaise, G. The space charge physics and the breakdown process. J. Appl. Phys. 1995, 77, 2916–2927. [CrossRef] Wang, X.; Yoshimura, N.; Murata, K.; Tanaka, Y.; Tanaka, T. Space-charge characteristics in polyethylene. J. Appl. Phys. 1998, 84, 1546. [CrossRef] Tanaka, T.; Montanari, G.C.; Mulhaupt, R. Polymer nanocomposites as dielectrics and electrical insulation-perspectives for processing technologies, material characterization and future applications. IEEE Trans. Dielectr. Electr. Insul. 2004, 11, 763–784. [CrossRef] Du, Y.F.; Lv, Y.Z.; Li, C.R.; Chen, M.T.; Zhong, Y.X. Effect of nanoparticles on electrical characteristics of transformer oil-based nanofluids impregnated pressboard. J. Appl. Phys. 2012, 111, 124322. [CrossRef] Energies 2017, 10, 1025 44. 45. 46. 47. 48. 49. 50. 51. 52. 53. 54. 55. 56. 57. 58. 59. 60. 61. 62. 63. 64. 65. 66. 67. 68. 20 of 21 Sartoratto, P.P.C.; Neto, A.V.S.; Lima, E.C.D.; de Sá, A.L.C.R.; Morais, P.C. Preparation and electrical properties of oil-based magnetic fluids. J. Appl. Phys. 2005, 97, 10Q917. [CrossRef] Li, J.; Zhang, Z.; Zou, P.; Grzybowski, S.; Zahn, M. Preparation of a vegetable oil-based nanofluid and investigation of its breakdown and dielectric properties. IEEE Electr. Insul. Mag. 2012, 28, 43–50. [CrossRef] Yang, Q.; Yu, F.; Sima, W.; Zahn, M. Space charge inhibition effect of nano-Fe3 O4 on improvement of impulse breakdown voltage of transformer oil based on improved Kerr optic measurements. AIP Adv. 2015, 5, 097207. [CrossRef] International Council on Large Electric Systems (CIGRE). Effect of Particles on Dielectric Strength; Working Group of 17 Committee: Paris, France, 2002. Lv, Y.Z.; Li, X.X.; Du, Y.F. Preparation and breakdown strength of TiO2 fluids based on transformer oil. In Annual Report Conference on Electrical Insulation and Dielectric Phenomena; IEEE: West Lafayette, IN, USA, 2010; pp. 1–3. Hong, R.; Pan, T.; Qian, J.; Li, H. Synthesis and surface modification of ZnO nanoparticles. Chem. Eng. J. 2006, 119, 71–81. [CrossRef] Selim, K.M.K.; Ha, Y.S.; Kim, S.J.; Chang, Y.; Kim, T.J.; Lee, G.H.; Kang, I.K. Surface modification of magnetite nanoparticles using lactobionic acid and their interaction with hepatocytes. Biomaterials 2007, 28, 710–716. [CrossRef] [PubMed] Bourlinos, A.B.; Bakandritsos, A.; Georgakilas, V.; Petridis, D. Surface Modification of ultrafine magnetic iron oxide particles. Chem. Mater. 2002, 14, 3226–3228. [CrossRef] Tsai, T.; Kuo, L.; Chen, P.; Lee, D.; Yang, C. Applications of ferronanofluid on a micro-transformer. Sensors 2010, 10, 8161–8172. [CrossRef] [PubMed] Si, S.; Li, C.; Wang, X.; Yu, D.; Peng, Q.; Li, Y. Magnetic Monodisperse Fe3 O4 Nanoparticles. Cryst. Growth Des. 2005, 5, 391–393. [CrossRef] Hwang, J.G.; Zahn, M.; O’Sullivan, F.; Pettersson, L.; Hjortstam, O.; Liu, R. Effects of nanoparticle charging on streamer development in transformer oil-based nanofluids. J. Appl. Phys. 2010, 107, 014310. [CrossRef] Du, Y.F.; Lv, Y.Z.; Li, C.R.; Chen, M.T.; Zhong, Y.X.; Zhou, J.Q.; Li, X.X.; Zhou, Y. Effect of semiconductive nanoparticles on insulating performances of transformer oil. IEEE Trans. Dielectr. Electr. Insul. 2012, 19, 770. OECD: Principles and Strategies Related to the Testing of Degradation of Organic Chemicals. Available online: http://www.oecd.org/chemicalsafety/testing/5598432.pdf (accessed on 1 April 2005). Methods for the Determination of the Lighting Imulse Breakdown Voltage of Insulating Liquids; IEC Standard 60897; IEC: Geneva, Switzerland, 1987. Metwally, I.A. Influence of Specimen Size on the Dielectric Strength of Transformer Oil. IEEE Trans. Electr. Insul. 1977, EI-12, 281–292. Maksjejewski, L.J.; Tropper, H. Some Factors Affecting the Measurement of the Electric Strength of Organic Liquids. Proc. IEEE 1954, 101, 183–190. Bartinikas, R. Electrical Insulating Liquids; ASTM Publication: Philadelphia, PA, USA, 1994. Zahn, M.; Ohki, Y.; Rhoads, K.; Lagasse, M.; Matsuzawa, H. Electro-optic charge injection and tramsport measurements in highly purified water and water/ethylene glycol mixtures. IEEE Trans. Dielectr. Electr. Insul. 1985, 20, 199. [CrossRef] Zhang, X.; Zahn, M. Kerr electro-optic field mapping study of the effect of charge injection on the impulse breakdown strength of transformer oil. Appl. Phys. Lett. 2013, 103, 162906. [CrossRef] Zahn, M.; Ohki, Y.; Fenneman, D.B.; Gripshover, R.J.; Gehman, V.H. Dielectric properties of water and water/ethylene glycol mixtures for use in pulsed power system design. Proc. IEEE 1986, 74, 1182. [CrossRef] Lewis, T.J. Interfaces: Nanometric dielectrics. J. Phys. D Appl. Phys. 2005, 38, 202. [CrossRef] Smith, R.C.; Liang, C.; Landry, M. The mechanisms leading to the useful electrical properties of polymer nanodielectrics. IEEE Trans. Dielectr. Electr. Insul. 2008, 15, 187. [CrossRef] Danikas, M.G. On two nanocomposite models: Differences, similarities and interpretational possibilities regarding Tsagaropoulos’ model and Tanaka’s Model. J. Electr. Eng. 2010, 61, 241. [CrossRef] Du, Y.F.; Lv, Y.Z.; Li, C.R.; Chen, M.T.; Zhou, J.Q.; Li, X.X.; Zhou, Y.; Zhong, Y.X. Effect of electron shallow trap on breakdown performance of transformer oil-based nanofluids. J. Appl. Phys. 2011, 110, 104104. [CrossRef] Missana, T.; Adell, A. On the applicability of DLVO theory to the prediction of clay colloids stability. J. Coll. Interface Sci. 2000, 230, 150–156. [CrossRef] [PubMed] Energies 2017, 10, 1025 69. 70. 71. 72. 73. 74. 75. 76. 77. 78. 79. 80. 81. 82. 83. 21 of 21 Popa, I.; Gillies, G.; Papastavrou, G.; Borkovec, A. Attractive and repulsive electrostatic forces between positively charged latex particles in the presence of anionic linear polyelectrolytes. J. Phys. Chem. B 2010, 114, 3170–3177. [CrossRef] [PubMed] Kudelcik, J.; Bury, P.; Kopcansky, P.; Timko, M. Dielectric breakdown in mineral oil ITO100 based magnetic fluid. Phys. Proced. 2010, 9, 78–81. [CrossRef] Li, Y.; Zhou, J.; Tung, S.; Schneider, E.; Xi, S. A review on development of nanofluid preparation and characterization. Powder Technol. 2009, 196, 89–101. [CrossRef] Yu, W.; Xie, H. A review on nanofluids: Preparation, stability mechanisms, and applications. J. Nanomater. 2012, 2012, 435873. [CrossRef] Wang, L.S.; Hong, R.Y. Synthesis, surface modification and characterization of nanoparticles. In Advances in Nanocomposites—Synthesis, Characterization and Industrial Applications; InTech: Suzhou, China, 2011; pp. 289–323. Peppas, G.D.; Bakandritsos, A.; Charalampakos, V.P.; Pyrgioti, E.C.; Tucek, J.; Zboril, R.; Gonos, I.F. Ultrastable Natural Ester-Based Nanofluids for High Voltage Insulation Applications. ACS Appl. Mater. Interface 2016, 8, 25202–25209. [CrossRef] [PubMed] Tijerina, J.T.; Narayanan, T.N.; Gao, G.; Rohde, M.; Tsentalovich, D.A.; Pasquali, M.; Ajayan, P.M. Electrically Insulating Thermal Nano-Oils Using 2D Fillers. ACS Nano 2012, 6, 1214–1220. [CrossRef] [PubMed] Hwang, J.G.; O’Sullivan, F.; Zahn, M.; Hjortstam, O.; Pettersson, L.A.A.; Liu, R. Modeling of streamer propagation in transformer oil-based nanofluids. In Proceedings of the Annual Report Conference on Electrical Insulation and Dielectric Phenomena (CEIDP’08), Quebec City, QC, Canada, 26–29 October 2008; pp. 361–366. Mergos, J.A.; Athanassopoulou, M.D.; Argyropoulos, T.G.; Dervos, C.T. Dielectric properties of nanopowder dispersions in paraffin oil. IEEE Trans. Dielectr. Electr. Insul. 2012, 19, 1502–1507. [CrossRef] Krajnik, P.; Pusavec, F.; Rashid, A. Nanofluids: Properties, applications and sustainability aspects in materials processing technologies. In Advances in Sustainable Manufacturing: Proceedings of the 8th Global Conference on Sustainable Manufacturing; Springer: Berlin, Germany, 2011; pp. 107–113. Kochetov, R.; Morshuis, P.H.F.; Smit, J.J.; Andritsch, T.; Krivda, A. Precautionary remarks regarding synthesis of nanocomposites. In Proceedings of the 32nd Electrical Insulation Conference (EIC’14), Philadelphia, PA, USA, 8–11 June 2014; pp. 51–54. Nemmar, A.; Hoet, P.H.; Vanquickenborne, B.; Dinsdale, D.; Thomeer, M.; Hoylaerts, M.F.; Vanbilloen, H.; Mortelmans, L.; Nemery, B. Passage of inhaled particles into the blood circulation in humans. Circulation 2002, 105, 411–414. [CrossRef] [PubMed] Geiser, M.; Rothen-Rutishauser, B.; Kapp, N.; Schürch, S.; Kreyling, W.; Schulz, H.; Semmler, M.; Im Hof, V.; Heyder, J.; Gehr, P. Ultrafine particles cross cellular membranes by nonphagocytic mechanisms in lungs and in cultured cells. Environ. Health Perspect. 2005, 113, 1555–1560. [CrossRef] [PubMed] Sutherland, J.W.; Kulur, V.N.; King, N.C.; von Turkovich, B.F. An experimental investigation of air quality in wet and dry turning. CIRP Ann. Manuf. Technol. 2000, 49, 61–64. [CrossRef] Baroli, B.; Ennas, M.G.; Loffredo, F.; Isola, M.; Pinna, R.; López-Quintela, M.A. Penetration of metallic nanoparticles in human full-thickness skin. J. Investig. Dermatol. 2007, 127, 1701–1712. [CrossRef] [PubMed] © 2017 by the authors. Licensee MDPI, Basel, Switzerland. This article is an open access article distributed under the terms and conditions of the Creative Commons Attribution (CC BY) license (http://creativecommons.org/licenses/by/4.0/).